IS : 2430-1986
SAMPLING OF AGGREGATES
( First Revision
Third Reprint SEPTEMBER 1993
BUREAU OF INDIAN STANDARD S
MANAKBHAVAN, 9 BAHADUFt SHAH ZAFARMARG
NEW DELHI 110002
Gr3 3wu 1987
( Reaffirmed 1995 )
SAMPLING OF AGGREGATES
( First Revision )
Building Materials and Components Sampling Sectional Committee,
DR MOEAN RAI
Central Building Research Institute ( CSIR ),
SIiRIS. K. Goswanr ( Al&safe to
Dr Mohan Rai )
SHRI S. K. BANERJEE National Test House, Calcutta
DR P. Ray CHAUDRURI Centgralhyd Research Institute ( CSIR ), New
SBRI L. A. GOKHALE Mini~;iykXwTransport, Department of Railways,
Sam B. K. JAIN ( Alfrmutr )
SHRI S. C. KUYAR Development Commiuioner, Small Scale Industries.
SHRI K. V. K. RAJU ( Allrmare )
SHRI M. V. LAKSF~XANASAMY Indian Statistical Institute, Calcutta
DR A. G. MADHAVA RAO Struc;;;iaFineering Research Centre ( CSIR ),
SHRI D. S. RAYACHANDRA
MURTHY ( Alinnate )
SHRI J. P. MAIKWRI
SHRI P. P. SAXENA ( Akrrnatc )
Export Inspection Council of India, New Delhi
DR A. K. MULLICK Nati~$“,t$l for Cement and Building Materiala,
SHRI K. H. BABU ( Alternate )
SERI S. S. RAJPUT
Forest Research Institute and Colleges. Dehra Dun
National Buildings Organization, New Delhi
SHRI T. R. BHATIA ( Akmutr )
SHRI N. VEERABADHU
SHRI S. B. JAISWAL ( Aftrrnotc )
Central Public Worka Department, New Delhi
SHRI G. VENXATESULU Ministry of Shipping and Transport, New Delhi
SHRI PRAFULLA KUMAB ( Afternate )
SHRX G. W. DATEY, Director General, BIS ( Ero@cio Mmbn )
Director ( Stat: )
SYT ANDPAM GUPTA
Deputy Director ( Stat ), BIS
@ Cowight 1987
BUREAU OF INDIAN STANDARDS
This publication is protected under the Indian Co@yriiht Act ( XIV of 1957) and
reproduction in whole or in part by any means except with written permission of the
publisher shall be deemed to be an infringement of copyright under the said Art.
IS : 2430- 1986
SAMPLING OF AGGREGATES
( First Revision
0.1 This Indian Standard ( First Revision ) was adopted by the Indian
Standards Institution on 28 November 1986, after the draft finalized by
the Building Materials and Components Sampling Sectional Committee
had been approved by the Civil Engineering Division Council.
0.2 Sampling is of equal importance to testing and a man drawing
samples shall use every precaution to obtain samples that will show the
true nature and condition of the materials which they represent.
0.3 One of the major contributing factors to the quality of concrete
is the quality of aggregates used therein. It is, therefore, imperative
that due consideration is given to sampling procedures which will help
in the proper and objective evaluation of the quality of aggregates.
0.4 This standard was originally issued in 1969. This has been revised
so as to make it more easily implementable in practice and bring it in
line with the current national and international trade practices. [ In
this revised version, the weight of the gross sample and number of
increments have been modified so that it may be more economical to
use them in practice.]
0.5 In preparing this standard, assistance has been derived from the
ASTM/D 75-1982 Standard practice for sampling aggregates
ISO/DIS 4847 Concrete - Sampling of normal weight aggregates.
0.6 For reporting the results of a test or analysis, if the final value,
observed or calculated, is to be rounded off, it shall be done in accordance
with IS : 2-1960*.
*Ruler for rounding off numerical values ( rsckad ).
E.,-..r I.._. - ._._ I___. “_._..
IS : 2430 - 1986
1.1 This standard prescribes the methods of sampling for coarse and
fine aggregates for the following purposes:
a) PreIiminary investigation of source of suppl’y,
b) Inspection of shipment of materials, and
c) Inspection of materials on the site of work.
1.2 This standard also specifies methods of sample reduction, packing
and forwarding them for examination and testing.
2.0 For the purpose of this standard, the following definitions shall
2.1 Aggregates - Crushed stone, crushed boulders, gravel, sand,
industrial by-products or such other inert material.
2.2 Fine Aggregates - Aggregates most of which pass thtough
4’75 mm IS Sieve.
2.2.1 Natural Sand - Fine aggregates resulting from the natural
disintegration of rock and which have been deposited by streams or
2.2.2 Crushed Stone Sand - Fine a’ggregates produced by crushing
2.2.3 Crushed Gravel Sand - Fine aggregates produced by crushing
2.3 Coarse Aggregates - Aggregates most of which are retained on
4’75 mm IS Sieve.
2.4 All-in Aggregates - Material composed of fine aggregates and
2.5 Lot - The quantity of aggregates of the same class, nominal size,
source and offered for inspection at one time. The lot may consist of
the whole or a part of the quantity ordered for.
2.6 Sub-lot - The quantity of aggregates in each of the parts into
which a lot is divided for the purpose of sampling. As far as possible
sub-lots should be of equal size.
2.7 Increment - The quantity of aggregates obtained by a sampling
device at one time.
2.8 Unit Sample - The quantity of aggregates collected at one point
in sectional -ampling or at one time from the conveyor.
IS : 2430 - 1986
2.9 Gross Sample - Sample as collected from a sub-lot, that is, the
quantity of aggregates consisting of one Or several increments or unit
samples taken from a sub-lot.
2.10 Laboratory Sample - The quantity of aggregates obtained by
reducing a gross sample following a specified procedure and intended
for laboratory testing.
2.11 Composite Sample ( for the Lot ) - The quantity of
aggregates obtained by mixing together equal quantities from each of
the laboratory samples.
3. SAMPLING FOR PRELIMINARY INVESTIGATION OF
SOURCE OF SUPPLY
3.1 Stone from Ledges for Quarries
3.1.1 The ledge or quarry face of the stone shall be inspected to
determine any discernible variations or strata. Differences in colour
and texture shall be observed.
3.1.2 Separate samples having a mass of at least 25 kg of stone should
be obtained from each discernible strata. The sample should not
include material weathered to such an extent that it is no longer useful
for the purpose intended.
3.2 Field Stone and Boulders
3.i.l A detailed inspection of the deposits of field stone and boulders,
over the area from where the supply is to be obtained, shall be made.
The different kinds of stone and their condition in various deposits shall
3.2.2 Separate samples shall be selected of all classes of stone that
visual examination indicates would be considered for use in construction.
These individual samples shall weigh at least 25 kg each.
3.3 Sand and Gravel ( Road Side, Bank Run Sand and Gravel
3.3.1 Road side production is the production of materials with
portable or semi-portable crushing, screening, or washing plants estab-
lished or reopened in the vicinity of the work on a designated project
for the purpose of supplying materials for that project.
3.3.2 Potential sources of bank run sand may include previously worked
pits from which there is an exposed face or potential deposits discovered
through air-photq, interpretation, geo-physical exploration or other
types of investigation.
3.3.3 Samples shall be so chosen from each of the different strata in
the deposit discernible to the sampler. An estimate of the quantity of
different materials shall be made.
IS : 2430 - 1986
3.3.4 If the deposit is worked as an open-face bank or pit, the sample
shall be taken by channelling the face vertically, top to bottom, so as
to represent the materials proposed for use. Over-burden and disturbed
material shall not be included in the sample. Test holes shall be
excavated or drilled at numerous locations in the deposit to determine
quality of material and the extent of the deposit ljeyocd the exposed
face, if any. The number and depth of these lest holes will depend
upon the quantity of the materia1 to be used, topography of the area,
nature of the deposit, character of the material and potential value of
the material in the deposit. Separate samI>les shall be obtained from
the face of the bank and from test holes. If visual inspection indicates
that there is considerable variation in material, indivii;ual samples shall
be selected from the material in each well defined stratum. Each sample
shall be thoroughly mixed and quartered, if necessary, so that the.gross
sample obtained wail be of at least 12 kg for sand and 33 kg If the
deposit contains an appreciable amount of coarse aggregates. If the
deposit being in,estiqated does not have an open face, sample shall
be obtained entirely from test holes as outlined herein.
4. SAMPLING FOR INSPECTION OF SHIPMENT OF
MATERIALS AND OF MATERIALS ON THE SITE OF
4.1 The samples shall be selected and examined from each lot ( see 2.5 )
4.1.1 For obtaining reliable conclusions, it is recommended that as
far as possible aggregates be sampled when in motion, that is, from
conveyors or during loading and unloading,
4.2 Sampling from Conveyors
4.2.1 Sub-lots - For the purpose of sampling a lot, while it is being
discharged over a conveyor, shall be divided into a number of sub-lots
of approximately equal size as specified in Table 1.
TABLE 1 NUMBER OF SUB-LOTS INTO WHICH A LOT IS
TO BE DIVIDED
( Clauses4.2.1, 4.3.1 and 4.4.3 )
LOT STZE No. OF SrjB-LOTS
101 to 500 3
501 to 1 500 5
I 501 to 5 000 7
NOTE - In case the lot contains 100 ms or less of aggregates, the sampling shall
be subject to agreement between the purchaser and the supplier.
IS :2430- 1986
22.214.171.124 A representative gross sample shall be drawn from each of
the sub-lots and shall be kept separately. Thus there will be as many
gross samples as the number of sub-lots into which the lot has been
4.2.2 The weight of the grocs sample shall depend on the maximum
nominal size of aggregates and shall be according to Table 2. In order
to obtain this weight of gross sample, at least 10 increments of a suitable
weight, each not less than 1 kg, shall be taken. Increments shall be
taken with the help of a suitable scoop ( see Fig. 1 ) at regular intervals.
TABLE 2 WEIGHT OF GROSS SAMPLE
M_cama NOMINAL SIZE OF MINIMUMWEIGHT OF
( kg )
NOTE 1 - For aggregates, the maximum nominal size of particles is the largest
sieve size upon which any material is permitted to be retained.
NOTE 2 -For all-in-aggregates, minimum weight of gross sample shall be the
mass of coarse aggregates ( minimum ) plus 10 kg.
Dimansions ofthe Scoopin mm
A B c D E
’10 250 250 120 200 300
5 200 200 90 175 240
2 150 150 75 125 180
FIG. 1 SAMPLINGShoop
IS : 2430 - 1986
126.96.36.199 The increments shall be taken at equal intervals preferably
from the cross section and thickness of the stream in one operation.
When the aggregates are in motion, the most reliable means of taking
such increments is to sample at a point where the material discharges
from the belt. The best possible increment is one which cuts across
entirely the falling steam of the material by means of a suitable
receptacle passed from one side of the steam to the other without
allowing the receptacle to overflow. If the whole of the steam cannot
be covered by one increment without overflowing the receptacle, the
steam should be sampled systematically by taking material from all
188.8.131.52 If’it is not possible to sample satisfactorily at the point of
discharge, increments may be drawn from the moving belt itself. In
this case, the increments shall be col1ecte.d from the centre and the
left and right side of the belt along the same width. To ensure that very
small material is also correctly obtained, a scoop should sweep the
4.2.3 The material collected from various increments in a sub-lot
shall be combined and mixed together to constitute a gross sample.
4.3 Sampling from Transportation Units ( Wagons, Trucks and
4.3.1 Sub-lots - For the purpose of sampling, all the carriers ( wagons/
trucks/boats ) in a lot shall be divided into a suitable number of sub-lots
of approximately equal size in accordance with the requirements of
184.108.40.206 A representative gross sample shall be drawn from each of
the sub-lots and shall be kept separately. Thus, there will be as many
gross samples as the number of sub-lots into which a lot has been
4.3.2 In order to get a representative gross sample, the aggregates
shall be sampled as far as possible when in motion, during loading or
220.127.116.11 A minimum of 25 percent of the carriers shall be selected
at random from the sub-lot. ‘For the random selection of carriers, the
procedure given in 3.1 of IS : 4905-1968” may be followed. Ten
increments shall be taken from the selected carriers and a suitable
weight of the increment, not less than 1 ks, shall be used SO that a
Fross sample of the quantity required m Table 2 is obtained. The
Increments shall be evenly distributed over the selected carriers with a
*Methods for random sampling.
IS : 2430 - 1986
view to determine the necessary number of increments that should
be ,collected from e&h of the carriers in the sub-lot ‘for making up the
grogs sample. These increments shall be drawn with the help of a
suitable scoop ( see Fig. 1 ) at regular intervals, at the time of loading
or unloading of the carriers.
4.3.3 When the samples are to be collected from the 1Qaded carriers,
for collecting ten required increments, an equal number of points shall
be located at random on the entire aggregate surface of all the carriers
in a sub-lot. At every selected point, an increment shall be collected by
the sectional sampling method.
18.104.22.168 Sectional sam/ding - At every selected point an increment shall
be collected by taking the whole section of’ aggregates from top to
bottom over the area of a circle of 20 cm diameter for aggregates more
than 20 mm nominal size. For doing so, aggregate from the surface up
to a depth of approximately 45 cm shall be collected at first. The
bottom of the hole so formed shall then be covered by a plate and the
aggregate lying on the sides shall be removed up to that plate so that,
when the hole is dug further, the material from the sides does not fill
up the hole by falling down. The procedure is repeated till the bottom
is reached. For aggregates up to 20 mm nominal size and fine aggre-
gates a sampling auger may be used in a casing pipe of 15 cm diameter
and length slightly more than the height of the sub-lot. The casing
pipe is pushed vertically down till it touches the bottom of the lot. The
entire material from the inside of the ca$ing pipe is removed by the
auger to give an increment.
22.214.171.124 In sampling coarse aggregates from loaded carriers effort
should be made to enlist’ the services of power equipment capable of
exposing the material at various levels and random locations. When
power equipment is not available the procedure given in 126.96.36.199 may
4.4 Sampling from Stacks or Stock Piles
4.4.1 For sampling material from stock piles or stacks, it is very
difficult lo ensure unbiased samples, due to the segregation which often
occurs when material is stacked, with coarser particles rolling to the
outside face of the pile. For coarse or all-in aggregates every effort
should be made to procure a power equipment to develop a separate,
small sampling pile composed of materials drawn from various levels
and locations in the main pile after which several increments may be
combined to compose the gross sample. If it is necessary to indicate
the degree of variability existing within the main pile, separate samples
should be drawn from separate areas of the pile.
4.4.2 Where power equipment is not available, samples from sack
piles should be made up of the required number of increments taken
equally from top third, at the mid point and at the bottom third of the
volume of the pile. A board put vertically into the pile just above the
sampling point helps in preventing further segregation. In sampling
stock piles of the aggregates, the outer layer which may have become
segregated, should be removed and the sample taken from the material
4.4.3 Sub-lots - For the purpose of sampling, the quantity of
aggregates in a stack shall be divided into a suitable number of sub-lots
of approximately equal size in accordance with Table 1.
188.8.131.52 A representative gross sample shall be drawn f;om each of
the sub-lots. Thus there will be as many gross samples as the number
of sub-lots into which the lot has been divided.
4.4.4 Sampling of aggregates from stacks shall be carried out as far
as possible, during the making ( or breaking ) of the stack.
184.108.40.206 A minimum of ten increments shall be taken from a sub-lot
for making up a gross sample. The weight of the gross sample shall be
according to Table 2 for various sizes of aggregates. The weight of
the increment shall be governed by the weight of the gross simple and
minimum number of increments i.e. 10. This weight of increment
shall not be less than 1 kg. The number of increments shall be equally
distributed over the sub-lot. Increments shall be drawn with the help
of a suitable scoop ( see Fig. 1 ) at regular intervals in the course of
making or unmaking of the stacks.
4.4.5 When it becomes necessary to sample a stationary stack, trench
sampling method ( see 220.127.116.11 and 18.104.22.168 ) may be used. This method
is applicable for stacks up to a maximum height of 1’5 m only.
22.214.171.124 The weight of the gross sample shall be according to
Tabfe 2 and minimum number of increments from a sub-lot shall be ten.
These increments shall be collected according to 126.96.36.199.
188.8.131.52 Along a randomly chosen line on the aggregates surface of
the sub-lot, a trench shall be dug right down to the ground level. From
the trenches so dug, the required number of increments shall be collected
with the help of a suitable sampling scoop ( see Fig. 1 ) at various
points randomly spread over the two exposed sides of the trenches. In
case of large stacks, in addition to the trench, the sides of the piles may
also be opened to expose the aggregates down to the bottom at places
where the trench does not expose the aggregates inside.
5. REDUCTION OF GROSS SAMPLE
5.1 Each gross sample shall be reduced separately. The process of
mixing and reduction of each gross sample shall be repeated until the
material required for each test, as specified in the relevant test method
specification, IS : 2386 ( Parts 1 to 8 )-1963* is obtained.
*For titles of the various parts of IS : 2386, see page 12.
IS : 2430 - 1986
5.2 Reduction by Riffle Divider - The aggregates shall be well mixed
and poured into the riffle. This process shall be repeated using different
size riffles according to the size of the aggregates.
5.3 Coning and Quartering Method - The aggregates shall be
mixed and then scooped into a cone-shaped pile. Care shall be taken
to drop each scoopful exactly over the same spot as otherwise the central
axis of the, cone will be slackened and an uneven distribution of the
particle sizes will result. After the cone is formed, it shall be flattened
by pressing the top of the cone with the smooth surface of the scoop.
Then it is cut into quarters by two lines which intersect at right angles
at the centre of the cone. The bulk of the sample is reduced by
rejecting any two diagonally opposite quarters. Accuracy in quartering
is most easily attained, in the case of fine and all-in-aggregates, with
6. PACKING AND MARKING OF SAMPLES
6.1 Each sample shall be packed separately and despatched to the
testing laboratory, great care being taken in packing to prevent the loss
of any fine material.
6.1.1 Coarse aggregates shall be packed in secure containers or sample
6.1.2 Fine aggregates and all-in aggregates shall be packed in tight
containers or closely woven bags so that there is no loss of the finer
642 Each package shall include a card, suitably protected from damage
by moisture and abrasion, giving the name and address of the sender
and the information required in 6.2.1.
6.2.1 As much as possible the following information about the origin
of the material shall accoinpany each sample:
a) Name of the quarry, pit, river-bed, etc, and address;
b) Proposed use for the material; and
c) Geographic location, and shipping facilities.
7. NUMBER OF TESTS AND REPORTING OF TEST RESULTS
7.1 Unless otherwise stated each sample shall be tested individually for
all the requirements and test results reported in accordance with
IS : 2386 ( Parts 1 to 8 )-1963*.
*For titles of the variousparts of IS : 2386, see page 12.
IS : 2430 - 1986
Titles of Various Parts of IS : 2&%X
IS : 2386 ( Part 1 )-I963
IS : 2386 (Part 2 )-1963
IS : 2386 ( Part 3 )-I963
IS : 2386 ( Part 4 )-I963
IS : 2386 ( Part 5 )-I963
IS : 2386 ( Part 6 )-1963
IS : 2386 ( Part 7 )-1963
IS : 2386 ( Part 8 )-1963
Methods of test for aggregates for concrete: Part 1 Particle
size and shape
Methods of test for aggregates for concrete: Part 2 Estimation
of deleterious materials and organic impurities
Methods of test for aggregates for concrete: Part 3 Specific
gravity, density, voids, absorption and bulking
Methods of test for aggregates for concrete: Part 4 Mechani-
Methods of test for aggregates for concrc te: Part 5 Soundness
Methods of test for aggregates for concrete: Part 6 Measuring
mortar making properties of fine aggregate
Methods of test for aggregates for concrete: Part 7 Alkali
Methods of test for aggregates for concrete: Part 8 Petro-
6lJREtiU OF INDIAN STANDARDS
Manak Bhavan, 9 Bahadur Shah Zafar Marg. NEW DELHI 110002
Telephones : 331 01 31 Telegrams : Manaksansthe
331 13 75 (Common to all Offices)
331 01 31
37 86 62
Regional Offices :
Central : Manak Bhavan, 9, Bahadur Shah Zafar Marg.
NEW DELHI 110002
l Eastern : l/l4 C.I.T. Scheme VII M,
V.I.P. Road, Maniktola. CALCUTTA 700054
Northern : SC0 445-446, Sector 35-C, CHANDIGARH 160036
: C.I.T. Campus, IV Cross Road, MADRAS 600113
: Manakalaya, E9 MIDC. Marol. Andheri (East),
Branch Offices :
‘Pushpak’, Nurmohamed Shaikh Marg. Khanpur, AHMADABAD 380001
t Peenya Industrial Area, 1st Stage, Bangalore-Tumkur Road,
Gangotri Complex, 5th Floor, Bhadbhada Road, T.T. Nagar. 55 40 21
Plot No, 82/83, Lewis Road, BHUBANESHWAR 751002 5 36 27
Kalai Kathir Bullding, 6/48-A Avanasi Road, COIMBATORE 641037 2 67 05
Quality Marking Centre. N.H. IV. N.I.T., FARIDABAD 121001 -
Savitri Complex, 116 G. T. Road, GHAZIABAD 201001 8-71 19 96
5315 Ward No. 29, R.G. Barua Road, 5th Bv-lane. 3 31 77
58-56C L. N. Gupta Marg. ( Nampally Station Road )
R14 Yudhister Marg, C Scheme. JAlPUR 302005 *
117/418 B Sarvodaya Nagar, KANPUR 208005
Plot No. A-9, House No. 561/63. Sindhu Nagar, Kanpur Roaa
Patliputra Industrial Estate, PATNA 800013
Distnct Industries Centre Complex. Bagh-e-Ali Maidan.
T. C. No. 14/1421. University P. O., Palayam.
Inspection Offices (With Sale Point) :
Pushpanjali. First Floor, 205-A West High Court Road.
Shankar Nagar Square, NAGPUR 440010
Institution of Engineers (India) Building. 1332 Shivaji Nagar.
41 29 16
6 32 92 95
2 63 48
39 49 55
6 34 71
21 68 76
5 56 07
6 2, 05
6 21 04
52 51 71
5 24 35
‘Sales Office Calcutta is at 5 Chowringhea Approach.
P. 0. Princep Street, CALCUTTA
t Sales Office is.at Novelty Chambers, Grant Road, BOMBAY
2 Sales. Office isat Unity Building, Narasimharaja Square,
27 68 00
89 65 28
Reprography Unit, BIS, New Delhi, India